 Nano Express
 Open Access
 Published:
Plasmonically induced perfect absorption in graphene/metal system
Nanoscale Research Letters volume 14, Article number: 300 (2019)
Abstract
The constructive interference of bright and dark plasmonic modes results in plasmoninduced absorption (PIA) effect. Here, we theoretically investigate PIA effect, which is realized by the constructive interference between a FabryPerot (FP) resonance mode and a graphene quasiguided mode. Numerical simulation reveals at least three advantages of our structure over previous ones. First, the extinction ratio can reach ~ 99.999%, resulting in the ultrahigh figure of merit* (FOM*) as high as 10^{6}. Second, the intensity of this pronounced PIA effect can be optimized by adjusting the coupling distance. Third, the resonance frequency can be easily tunable by tuning the graphene Fermi level. This system may have potential applications in dynamically optical switching and biochemical sensing.
Background
Plasmonics has attracted wide attention due to its extraordinary properties [1,2,3,4,5,6,7,8,9,10,11,12,13,14,15] and huge potential in many fields, including integrated photonics, biosensing, energy capture, photodetection. Recently, a novel plasmonic phenomenon, known as the spoof surface plasmons (SSPs), has been observed, which can propagate through perforated metals and overcome the diffraction limit [16]. SSPs were then explored in the THz, microwave, and lower frequency range [17,18,19], and a number of deepsubwavelength devices based on SSPs have been proposed demonstrated [20, 21]. However, the application of such devices is seriously hampered by SPPs’ high damping rate. One solution to this issue is the artificial plasmoninduced transparency (PIT) medium [22], which features a sharp transparency window within a broad absorption spectrum. The PIT effect mainly relies on the coupling of a radiative element and a subradiant element, which has been widely studied [23,24,25]. A similar phenomenon, plasmoninduced absorption (PIA), has also been demonstrated recently, which results from the constructive interference of bright and dark plasmonic modes [26]. The PIA resonance [27, 28] can exhibit remarkably fastlight effect, which has potential applications in optical switching and processing.
However, traditional devices based on the PIA effect of the metallic structure are hard or impossible to obtain tunability, which seriously restricts its applications. Graphene [29, 30], known for its semimetallicity, high mobility, and high tunability, can be an excellent candidate material for tunable infrared plasmonic devices. In this paper, we investigated a tunable PIA effect, which is achieved by the constructive interference of an FP resonance mode and a quasiguided mode supported by a periodic silver groove and monolayer graphene respectively. It is found that the resonance strength and linewidth are strongly dependent on coupling distance. It is also shown that the extinction ratio can reach ~ 99.999%. The extinction ratio is defined as 1RT, where R and T are the reflectance and transmittance, respectively. It is simply 1R in our system since the transmittance here is 0. As a result, an ultrahigh FOM* as high as 10^{6} in the graphene/metal system can be achieved and the resonance frequency can be dynamically tunable by adjusting the gate voltage of graphene. These prominent properties can be applied in biochemical sensing and dynamically optical switching.
Methods
The schematic of our structure is shown in Fig. 1, consisting of a monolayer graphene and an Al_{2}O_{3} isolated layer on top of a grooved silver. The thickness of the Al_{2}O_{3} is g. The system is illuminated by a normalincident plane wave of transverse magnetic (TM) polarization. The other structural parameters are expressed as follows: d is the depth of the silver groove; w is the width of the silver groove; P is the period of the unit cell. In the midinfrared region, intraband scattering dominates in highly doped graphene, and its conductivity takes on a Drudelike form σ_{g} = ie^{2}E_{F}/[πħ^{2}(ω+iτ^{1})]. The electron relaxation time is expressed as τ = μE_{F}/eυ_{F}^{2}, where υ_{F} = c/300 is the Fermi velocity, E_{F} is the Fermi energy and μ = 10 m^{2}/Vs is the DC mobility of graphene [25, 31, 32]. In the finitedifference timedomain (FDTD) simulations, the optical constants for silver, and Al_{2}O_{3} are from ref. [33] and ref. [34]. The periodic boundary conditions are used to simulate infinite periodic cell structures. For simplicity, we assume the material of the region above the graphene layer is vacuum (ε_{0} = 1).
Results and Discussion
We simulated the reflection spectrum of the silver groove with w = 100 nm, P = 250 nm, d = 2000 nm, and the result is shown in Fig. 2a (red curve). A wide dip can be observed at ~ 28 THz, with an extinction ratio ~ 44% and Q factor ~ 0.8, which is due to an FP resonance induced by the SSP excited by incident light [19]. This resonance has a wide range of resonance bands and thus the resonance mode can serve as the superradiant mode in our PIA system. Then, we calculated the reflection spectrum of the graphene sheet with metal boundary conditions in the bottom of the simulation area, with a Fermi level E_{F} = 0.3 eV, as shown in Fig. 2a (blue curve). The reflection spectrum shows that the graphene plasmon resonance can not be directly excited by the incidence at this frequency. To visualize and optimize the plasmon mode supported by the graphene, we first simulate the resonance modes supported by the graphene. To eliminate the potential impact of the silver groove’s FP resonance, we assume the groove is made of silicon instead of silver. The reflectance spectra of the structure were calculated for E_{F} = 0.3 eV and different unit cell P and is shown in Fig. 2b. A reflectance dip at resonant frequency f = 32.84 THz can be observed for P = 250 nm with a Q factor ~ 304. The high Q resonance with a narrow resonance band can serve as the subradiant (dark) mode in our PIA system. The reflectance dip is due to the resonance of plasmonic quasiguided mode in graphene with the normal incidence [35] since the groove can compensate the wavevector mismatch based on the mth order phasematching condition [36, 37]
where k_{x} = k_{0}sinθ, k_{0} = 2π/λ is the wavevector in free space, θ is the angle between the incident light and ydirection, n_{eff} is the effective refractive index of TM waveguide mode in the graphene, and G_{x} is the reciprocal lattice vector of the grating (G_{x} = 2π/P). In the following discussion, the incident light angle of ydirection is zero (θ = 0°). The situation for other incident angles is discussed in Additional file 1. The positions of these reflectance dips correspond to the resonance frequency of the quasiguided mode in the graphene, as shown in Fig. 2b. The simulation results agree well with the Eq. (1), where m = 1 and the effective refractive index, ~ 33, is obtained by FDTD solutions, as shown in Fig. 2c. The electric field E_{x} distributions of FP mode and graphene quasiguided mode have been shown in Fig. 2d. It is noted that the energy confinement of the SSP modes sustained by the Si grooved surface can be negligible compared with the graphene quasiguided mode.
In the coupling situation, the two eigenmodes will be strongly coupled when they get close to each other, and hence the reflection spectrum will be dramatically changed. A narrow, sublinewidth dip of enhanced absorbance with an extinction ratio ~ 99.97% is observed on top of the broader reflectance dip, as shown in Fig. 3a. When increasing the vertical distance g, the nearfield coupling and the quasiguided mode become weaker, as the modulation of the reflectance dip becomes smaller. There are two possible ways caused the reflectance dip smaller what are the weaker coupling and the weaker quasiguided mode excitation. Therefore, we used the coupled oscillator model to quantitatively understand the PIA system [38].
Where \( {\tilde{a}}_{1,2}={a}_{1,2}\left(\omega \right){\mathrm{e}}^{i\omega t} \), ω_{1,2} and γ_{1,2} are the timeharmonic amplitudes, resonant frequencies, and damping constants of the bright mode and the dark mode, respectively. b is the coupling coefficient measuring how strong the bright mode couples with the incident electric field. \( \tilde{\kappa}=\kappa {e}^{i\varphi} \) is a complex coupling parameter, which is introduced to express the phase retardation effect. φ is a phase shift, which is a key coefficient to determine the form of the interference between the two coherent pathways. When φ = 0 is a real parameter and the typical behavior of the PIT effect can be observed, and the interference between the two coherent pathways is destructive. For φ = π/2 is a pure imaginary parameter and the interference between the two coherent pathways is converted from destructive to constructive [26]. The absorption of the system can be calculated as the dissipated energy on the basis of formula (2), which is
Then, we fit the numerical absorption spectra with the Eq. (3) for different g, which have been shown in Fig. 3b (red curves). The simulation results are in good agreement with the analytical modeling results based on the coupled oscillator model, which strongly confirms the design principle of our PIA device. The fitting parameters κ, φ, γ_{1}, and γ_{2} have been shown in Fig. 4a–c. The increasing g yields a decrease in the coupling parameter κ, as shown in Fig. 4a. When gradually decreasing the coupling (increasing g), the phase φ is unchanged, and γ_{2} gradually decreases while γ_{1} changes slightly shown in Fig. 4b, c. The coupling parameter κ exceed the damping constants of dark mode γ_{2} for the minimum gap distance, which confirms that the coupling from the bright mode to the dark mode is stronger than the dissipation processes in the graphene sheet.
To visualize the constructive interference between the bright and dark modes, we investigated the structure’s magnetic field evolution with the time, and two H_{z} monitors have been placed 3 nm away from the center of graphene and 1000 nm away from the bottom of the silver groove, respectively. The oscillating phase difference between the two modes is 0.5π, as indicated in Fig. 5a. The magnetic field distribution at a different time was calculated in the PIA resonance frequency f_{q} = 32.5 THz, where ω_{q}t_{1} ~ 2.00 π and ω_{q}t_{2} ~ 2.50π, as indicated in Fig. 5b, c. The maximum of the magnetic field in the silver groove can be observed for 2.00π while the magnetic field in graphene reaches its maximum for 2.50π, indicating the outofphase coupling between the two structures. Therefore, the evolution and formation of the resonance are determined by constructive interference [39].
In practical application, a narrow reflection band and high extinction ratio are highly desired. To achieve these two conditions, we can adjust period of unit P and depth of silver groove d to optimize our structural parameters. After calculating the reflection spectrum of different structure parameters P from 1900 to 2100 nm and d from 245 to 265 nm by FDTD, we earn a very high extinction ratio ~ 99.999% in P = 254 nm and d = 1980 nm. The reflectance spectrum of the PIA device under different refractive index environments is shown in Fig. 6a. The sensing capabilities are defined as [39]:
where f and I are the resonance frequency and the spectral intensity, respectively. When measuring the reflection intensity of a sensor, the sensitivity capability of the sensor can be quantified by the FOM* value. The higher the value means the higher the sensitivity of the sensor. From Fig. 6 a, we can get S = 11.2 THz/RIU and the associated FOM~94.1, with the full width at half maximum (FWHM) ~ 30 nm (0.12 THz). This FOM is larger than the value in metamaterial absorbers based on surface lattice resonance. Also, our PIA sensor can lead to an ultrahigh FOM* value 3.5 × 10^{6}, as indicated in Fig. 6b. We compared the performance of the recently studied sensors in Additional file 1: Table S1.
In the PIA system, graphene plays another key role. The modulation of the resonant frequency can be achieved by tuning the gating voltage to adjust the Fermi level of graphene. The simulated spectra are shown in Additional files 2: Figure S1 and 3: Figure S2. The frequencyshift active control of the PIA resonance is meaningful for sensor or absorber.
Conclusions
In summary, we have numerically demonstrated the perfect absorption induced by constructive interference between FP resonance mode and graphene plasmonic quasiguided mode. Through the introduction of graphene plasmonic quasiguided mode, we obtain the spectral line with a narrower linewidth of the silver groove FP resonance mode. When the distance g is gradually increased, the resonance strength and linewidth will decrease. For the application, the FOM* in our system can achieve 10^{6}. Furthermore, the absorption window can be tuned by varying the geometrical parameter and the graphene Fermi level. These results could provide a new way toward the realization of nanoscale midinfrared dynamical spectral control and ultrasensitive optical sensors.
Availability of Data and Materials
All data generated or analyzed during this study are included in this published article [and its supplementary information files].
Abbreviations
 FDTD:

Finitedifference timedomain
 FOM*:

Figure of merit*
 FP:

FabryPerot
 FWHM:

Full width at half maximum
 PIA:

Plasmoninduced absorption
 PIT:

Plasmoninduced transparency
 Q factor:

Quality factor
 SSPs:

Spoof surface plasmons
 TM:

Transverse magnetic
References
 1.
Barnes WL, Dereux A, Ebbesen TW (2003) Surface plasmon subwavelength optics. Nature:824. https://doi.org/10.1038/nature01937
 2.
Liu GD, Zhai X, Wang LL, Lin Q, Xia SX, Luo X, Zhao CJ (2017) A Highperformance refractive index sensor based on Fano resonance in Si splitring metasurface. Plasmonics:1–5. https://doi.org/10.1007/s1146801604789
 3.
Shang XJ, Zhai X, Li XF, Wang LL, Wang BX, Liu GD (2016) Realization of graphenebased tunable plasmoninduced transparency by the dipoledipole coupling. Plasmonics:419–423
 4.
Xia SX, Zhai X, Wang LL, Lin Q, Wen SC. Excitation of crest and trough surface plasmon modes in inplane bended graphene nanoribbons (vol 24, pg 427, 2016). Opt Express 2016;7436
 5.
Qin M, Wang LL, Zhai X, Chen DC, Xia SX. Generating and manipulating high quality factors of Fano resonance in nanoring resonator by stacking a half nanoring. Nanoscale Res Lett 2017;doi: Artn 578 https://doi.org/10.1186/S1167101723575
 6.
Sun H, Zhu YC, Gao B, Wang P, Yu YT (2017) Polarizationdependent quasifarfield superfocusing strategy of nanoringbased plasmonic lenses. Nanoscale Res Lett. https://doi.org/10.1186/S1167101721541
 7.
Wang LD, Zhang T, Zhang XY, Song YJ, Li RZ, Zhu SQ (2014) Optical properties of Ag nanoparticlepolymer composite film based on twodimensional Au nanoparticle array film. Nanoscale Res Lett. https://doi.org/10.1186/1556276x9155
 8.
Sun L, Lin H, Kohlstedt KL, Schatz GC, Mirkin CA (2018) Design principles for photonic crystals based on plasmonic nanoparticle superlattices. Proc Nat Acad Sci USA:7242–7247. https://doi.org/10.1073/pnas.1800106115
 9.
Sang T, Gao J, Yin X, Qi H, Wang L, Jiao H (2019) Angleinsensitive broadband absorption enhancement of graphene using a multigrooved metasurface. Nanoscale Res Lett. https://doi.org/10.1186/s1167101929377
 10.
Zhang B, Li H, Xu H, Zhao M, Xiong C, Liu C, Wu K (2019) Absorption and slowlight analysis based on tunable plasmoninduced transparency in patterned graphene metamaterial. Optics Express:3598–3608. https://doi.org/10.1364/oe.27.003598
 11.
Xu H, Zhao M, Zheng M, Xiong C, Zhan B, Peng Y, Li H (2019) Dual plasmoninduced transparency and slow light effect in monolayer graphene structure with rectangular defects. J Phys DAppl Phys. https://doi.org/10.1088/13616463/aae9cc
 12.
Xu H, Xiong C, Chen Z, Zheng M, Zhao M, Zhang B, Li H (2018) Dynamic plasmoninduced transparency modulator and excellent absorberbased terahertz planar graphene metamaterial. J Opt Soc Am BOpt Phys:1463–1468. https://doi.org/10.1364/josab.35.001463
 13.
Kong XT, Khorashad LK, Wang Z, Govorov AO (2018) Photothermal circular dichroism induced by plasmon resonances in chiral metamaterial absorbers and bolometers. Nano Lett:2001–2008. https://doi.org/10.1021/acs.nanolett.7b05446
 14.
Yu P, Besteiro LV, Wu J, Huang Y, Wang Y, Govorov AO, Wang Z (2018) Metamaterial perfect absorber with unabated sizeindependent absorption. Opt Express:20471–20480. https://doi.org/10.1364/oe.26.020471
 15.
Atabaev TS (2018) Plasmonenhanced solar water splitting with metal oxide nanostructures: a brief overview of recent trends. Front Mater Sci:207–213. https://doi.org/10.1007/s1170601804134
 16.
Garciavidal FJ, Martínmoreno L, Pendry JB (2005) Surfaces with holes in them: new plasmonic metamaterials. J Opt A Pure Appl Op:S97
 17.
Hibbins AP, Evans BR, Sambles JR (2005) Experimental Verification of Designer Surface Plasmons. Science 670
 18.
FernandezDominguez AI, Williams CR, GarciaVidal FJ, MartinMoreno L, Andrews SR, Maier SA (2008) Terahertz surface plasmon polaritons on a helically grooved wire. Appl Phys Lett
 19.
Huang XR, Peng RW, Fan RH (2010) Making metals transparent for white light by spoof surface plasmons. Phys Rev Lett
 20.
Xiao B, Kong S, Xiao S (2016) Spoof surface plasmon polaritons based notch filter for ultrawideband microwave waveguide. Opt Comm:13–17
 21.
Gao Z, Gao F, Xu H, Zhang Y, Zhang B (2016) Localized spoof surface plasmons in textured open metal surfaces. Opt Lett:2181
 22.
Zhang S, Genov DA, Wang Y, Liu M, Zhang X (2008) Plasmoninduced transparency in metamaterials. Phys Rev Lett:047401
 23.
Liu SD, Yang Z, Liu RP, Li XY (2011) Plasmonicinduced optical transparency in the nearinfrared and visible range with double split nanoring cavity. Opt Express:15363–15370
 24.
Zeng C, Guo J, Liu X. Highcontrast electrooptic modulation of spatial light induced by grapheneintegrated FabryPérot microcavity. Appl Phys Lett 2014;1211035
 25.
Wang L, Li W, Jiang X (2015) Tunable control of electromagnetically induced transparency analogue in a compact graphenebased waveguide. Opt Lett:2325
 26.
Taubert R, Hentschel M, Kästel J, Giessen H (2012) Classical analog of electromagnetically induced absorption in plasmonics. Nano Lett:1367–1371
 27.
Li HJ, Wang LL, Zhai X (2016) Plasmonically induced absorption and transparency based on MIM waveguides with concentric nanorings. IEEE Photonics Technol Lett:1454–1457
 28.
Lin Q, Zhai X, Wang LL, Luo X, Liu GD, Liu JP, Xia SX (2016) A novel design of plasmoninduced absorption sensor. Appl Phys Express:062002
 29.
Xia SX, Zhai X, Wang LL, Sun B, Liu JQ, Wen SC (2016) Dynamically tunable plasmonically induced transparency in sinusoidally curved and planar graphene layers. Opt Express:17886–17899
 30.
Xia SX, Zhai X, Huang Y, Liu JQ, Wang LL, Wen SC (2017) Multiband perfect plasmonic absorptions using rectangular graphene gratings. Opt Lett:3052–3055
 31.
Lin Q, Zhai X, Wang L, Wang B, Liu G, Xia S (2015) Combined theoretical analysis for plasmoninduced transparency in integrated graphene waveguides with direct and indirect couplings. Epl:34004
 32.
Wang B, Zhang X, Yuan X, Teng J (2012) Optical coupling of surface plasmons between graphene sheets. Appl Phys Lett:131111–131114
 33.
Palik ED. Handbook of Optical Constants of Solids. Orlando: Academic Press; 1985. p185
 34.
Li Y, An B, Jiang S, Gao J, Chen Y, Pan S (2015) Plasmonic induced tripleband absorber for sensor application. Opt Express:17607
 35.
Gao W, Shu J, Qiu C, Xu Q (2012) Excitation of plasmonic waves in graphene by guidedmode resonances. Acs Nano:7806–7813
 36.
Hu C, Wang L, Lin Q, Zhai X, Ma X, Han T, Du J (2016) Tunable double transparency windows induced by single subradiant element in coupled graphene plasmonic nanostructure. Appl Phys Express 9:052001
 37.
Liu JT, Xu BZ, Hu HF, Zhang J, Wei X, Xu Y, Song GF (2013) Tunable couplinginduced transparency band due to coupled localized electric resonance and quasiguided photonic mode in hybrid plasmonic system. Opt Express:13386–13393
 38.
Taubert R, Hentschel M, Giessen H (2013) Plasmonic analog of electromagnetically induced absorption: simulations, experiments, and coupled oscillator analysis. J Opt Soc Am B Opt Phys:3123–3134
 39.
Liu N, Mesch M, Weiss T, Hentschel M, Giessen H (2010) Infrared perfect absorber and its application as plasmonic sensor. Nano Lett 10:2342
Acknowledgements
Not applicable.
Funding
This work was supported by the National Natural Science Foundation of China (grant nos. 61505052, 61176116, 11074069, and 61775055).
Author information
Affiliations
Contributions
CH, QL, MTW, and XZ designed the study and analyzed the data. LLW and XZ supervised the writing of the manuscript. All the authors have read and approved the final manuscript.
Authors’ Information
Not applicable.
Corresponding author
Correspondence to Xiang Zhai.
Ethics declarations
Competing Interests
The authors declare that they have no competing interests.
Additional information
Publisher’s Note
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Additional files
Additional file 1:
Table S1. The compare of the recent relevant works. (DOCX 19 kb)
Additional file 2:
Figure S1. The reflectance spectra of the graphenesilver groove structure at different incident angle θ. (PNG 236 kb)
Additional file 3:
Figure S2.The reflectance spectra of the structure of graphenesilver groove in normal incidence for different Fermi energy of the graphene sheet. (PNG 523 kb)
Rights and permissions
Open Access This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
About this article
Cite this article
Hu, C., Lin, Q., Zhai, X. et al. Plasmonically induced perfect absorption in graphene/metal system. Nanoscale Res Lett 14, 300 (2019). https://doi.org/10.1186/s1167101931219
Received:
Accepted:
Published:
Keywords
 Plasmonically induced absorption
 Graphene
 Perfect absorption